- THE MAGAZINE
- Advertiser Index
- Raw & Manufactured Materials Overview
- Classifieds & Services Marketplace
- Buyers' Connections
- List Rental
- Market Trends
- Material Properties Charts
- Custom Content & Marketing Services
- CI Top 10 Advanced Ceramic Manufacturers
- Virtual Supplier Brochures
Even when pottery has dried out in the studio for months or years, it still contains the atmospheric moisture of the surrounding environment. In this sense, the pottery is never really dry at this stage.
Moist clay goes through several important steps in the bisque firing process:
212 to 392°F
When pottery is heated in this temperature range, mechanical water (which is found on the particle surfaces of the clay) is driven off. When fast-firing occurs during this period, water can go off as high-pressure steam, causing a crack in the clay.
842 to 1112°F
The clay body goes through other changes, but the period from 212°F to approximately 1000°F (dull red heat in the kiln) statistically produces the greatest number of defects from fast-firing the bisque kiln.
At any point during these temperature ranges, the pottery can crack if fired too fast. The question then becomes: How fast is too fast? As a general guideline for most functional pottery forms not over 14 in. in height and/or thicker than ¼ in., a total firing time of 14 hours to cone 06 (1828°F) is recommended. Larger ceramic forms or sculpture that exceeds these dimensions should be bisque fired longer. Keep in mind that a longer bisque firing to prevent possible cracking poses no danger.